TOOLING APPLICATION HOT WORK TOOLING 1
UDDEHOLM TOOL STEELS FOR
TOOLING APPLICATION HOT WORK TOOLING2
This information is based on our present state of knowledge and is intended to provide
general notes on our products and their uses. It should not therefore be construed as a
warranty of specific properties of the products described or a warranty for fitness for a
Classified according to EU Directive 1999/45/EC
For further information see our “Material Safety Data Sheets”.
Edition 4, 10.2017
© UDDEHOLMS AB
No part of this publication may be reproduced or transmitted for commercial
purposes without permission of the copyright holder.
TOOLING APPLICATION HOT WORK TOOLING 3
Hot forging of metals 4
Warm forging 7
Progressive forging 8
Effect of forging parameters on die life 10
Die design and die life 11
Requirements for die material 14
Manufacture and maintenance of forging die 16
Surface treatment 17
Tool steel product programme
– general description 19
– chemical composition 20
– quality comparison 20
Tool steel selection chart 21
Cover illustration: Connecting rod forging tool.
Most of the photos are coming from Arvika Smide AB, Sweden and Fiskars Brands Finland Oy Ab
Selecting a tool steel supplier is a key decision for all parties, including the tool
maker, the tool user and the end user. Thanks to superior material properties,
Uddeholm’s customers get reliable tools and components. Our products are always
state-of-the-art. Consequently, we have built a reputation as the most innovative
tool steel producer in the world.
Uddeholm produce and deliver high quality Swedish tool steel to more than 100,000
customers in over 100 countries.
Wherever you are in the manufacturing chain, trust Uddeholm to be your number one
partner and tool steel provider for optimal tooling and production economy.
TOOLING APPLICATION HOT WORK TOOLING4
In hot forging a heated up billet is pressed
between a die set to a nearly finished product.
Large numbers of solid metal parts are pro-
duced in aluminium alloys, copper alloys, steel
or super-alloys where irregular shapes need to
be combined with good mechanical properties.
The main methods of drop forging are hammer
forging and press forging.
Hammer forging is characterized by a very short
contact time and very rapid rate of increase of
force with time (impact loading). The cumulative
contact time for the bottom die can be fairly long
if one includes the time between blows. How-
ever, since a lubricant with “blow-out” effect is
normally used with hammers, effective contact
between the part and the die only occurs during
the actual forging blow.
These features imply that impact toughness
and ductility are important properties for die
steel to be used in hammer dies. This does not
mean to say that wear resistance is not impor-
tant, particularly in smaller dies, which in fact
normally fail as a result of wear. In hammer forg-
ing, there is a lot to be said for using inserts of
a more wear-resistant die steel which are shrink
fitted into a tough holder material.
For larger, high-production hammer dies,
which may be resunk a number of times, it is
important that the die steel used has sufficient
hardenability that the later cavities are not sunk
in softer material with inferior wear resistance.
In press forging, the contact time under pres-
sure is much longer, and the impact load is
much lower than in hammer forging. In general
terms, this means that the heat resistance and
elevated temperature wear resistance of the die
steel are relatively more important than the
ability to withstand impact loading. However,
one must optimize impact toughness and
ductility in relation to wear resistance; this
applies particularly for large press dies which
are not supported from the sides. Since the
surface temperature of press dies will during
TOOLING APPLICATION HOT WORK TOOLING 5
Forging dies might fail as a result of some form
of gross cracking. This may occur during a sin-
gle cycle or, as is most common, over a number
of cycles; in the latter instance, the crack growth
proceeds via a high-stress fatigue mechanism.
Gross cracking is more frequent in hammer
blocks than in press tooling, because of the
greater degree of impact.
If all other damage mechanisms are sup-
pressed, a forging die will ultimately wear out
(parts out of tolerance). Wear occurs when the
work material plus oxide scale glide at high
velocity relative to the cavity surface under the
action of high pressure. It is most pronounced
at convex radii and in the flash land. Wear is
increased drastically if the forging temperature
is reduced (higher flow stress for the work
material). The explosion which occurs via com-
TYPICAL DIE FAILURES
The deterioration of forging dies is usually
associated with several processes which may
operate simultaneously. However, one of these
normally dominates and is the ultimate cause of
failure. In general, four distinct damage mecha-
nisms can be distinguished:
• mechanical fatigue and gross cracking
• plastic deformation
• thermal fatigue cracking (heat checking)
Different damage mechanisms can dominate in
different parts of the cavity.
Thermal fatigue Wear Wear
bustion of oil-based lubricant in the confined
space between forging and die can also give
rise to a type of erosive wear.
Thermal Cracking Wear Plastic
service generally be higher than for hammer
dies, it is important that the die surface is not
excessively chilled by lubrication. Otherwise,
premature heat checking or even thermal shock
cracking may result.
TOOLING APPLICATION HOT WORK TOOLING6
Gross cracking is a failure condition which can
almost always be rectified. Normally, cracking lies in
one or more of the following:
• overloading, e.g. work material temperature
• die design, e.g. too sharp radii or too thin wall
• inadequate preheating of the die
• inadequate toughness of die steel (wrong
• too high hardness of die material
• poor quality heat treatment/surface treatment
• inadequate die support/alignment
This occurs when the die is locally subjected to
stresses in excess of the yield strength of the
die steel. Plastic deformation is quite common
at small convex radii, or when long thin tooling
components e.g. punches, are subjected to high
The following can be the cause of plastic
deformation in forging dies:
• too low billet temperature (high flow stress of
• inadequate hot strength of die steel
• die temperature too high
• die material too soft
Totally cracked die.
THERMAL FATIGUE CRACKING
This results if the surface of the cavities is
subjected to excessive temperature changes
during the forging cycle. Such temperature
changes create thermal stresses and strains at
the die surface which eventually lead to cracking via
a low-cycle fatigue mechanism (heat checking).
Thermal fatigue cracking is increased by the
• cavity surface at too high temperature
(excessive billet temperature and/or long
• excessive cooling of die surface between
• inadequate preheating of die
• wrong selection of die steel and/or poor heat
All these factors will increase the difference
between maximum and minimum temperature in
the die surface.
TOOLING APPLICATION HOT WORK TOOLING 7
Warm forging is a precision forging operation
carried out at a temperature range between
550–950°C (1020–1740°F). It is useful for forg-
ing of details with intricate shapes, with desir-
able grain flow, good surface finish and tighter
dimensional tolerances than if hot forged.
The weight of the forged piece is between
0.1–50 kg (0.22–110 lbs) and the production rate
about 10–40 pieces per minute. The contact time
is about 200 ms and the mechanical loads at 600°C
(1110°F) are 3 to 5 times higher than in hot forging.
Automatic multistation presses with integrated
cooling/lubricating systems are often used.
OPEN DIE EXTRUSION
Typical processes in warm forging.
DIE MATERIAL PROPERTIES
The properties profile required for tool steel in
forging dies depends to some extent on the
type of forging operation, on the work material
and on the size of the part, depth of cavity etc.
However, a number of general characteristics
will always be required in all forging operations.
The particular die damage mechanism are given
• Sufficient hardness and ability to retain this at
elevated temperatures—temper resistance
(wear, plastic deformation, thermal fatigue
• Enhanced level of hot tensile strength and hot